# this file is part of refractiveindex.info database
# refractiveindex.info database is in the public domain
# copyright and related rights waived via CC0 1.0

REFERENCES: "<a href=\"http://refractiveindex.info/download/data/2017/ohara_2017-11-30.agf\">OHARA Zemax catalog 2017-11-30</a> (obtained from <a href=\"http://www.ohara-inc.co.jp/en/product/optical/list/\">http://www.ohara-inc.co.jp</a>)<br>See also <a href=\"http://refractiveindex.info/download/data/2017/ohara_2017-11-30.pdf\">OHARA glass data sheets</a>"
COMMENTS: ""
DATA:
  - type: formula 3 
    range: 0.3 2.4
    coefficients: 2.5432134 -0.0102068 2 0.013983216 -2 0.00045963235 -4 -3.2963243e-05 -6 1.9413424e-06 -8
  - type: tabulated k
    data: |
        0.300 5.7485E-06
        0.310 3.5206E-06
        0.320 2.1492E-06
        0.330 1.2981E-06
        0.340 7.4253E-07
        0.350 4.2007E-07
        0.360 2.3265E-07
        0.370 1.3865E-07
        0.380 8.5878E-08
        0.390 6.2700E-08
        0.400 4.1652E-08
        0.420 2.6846E-08
        0.440 2.4596E-08
        0.460 2.2030E-08
        0.480 1.5310E-08
        0.500 1.1955E-08
        0.550 8.7623E-09
        0.600 1.4345E-08
        0.650 1.5541E-08
        0.700 1.6736E-08
SPECS:
    n_is_absolute: false
    λ_is_vacuum: false
    temperature: 25.0 °C
    coefficients_of_thermal_dispersion: 2.929e-06 0.0 0.0 0.0 0.0 0.0
    n_d: 1.607291
    V_d: 59.375631
    glass_code: 607594
    glass_status: preferred
    density: 3.51 g/cm<sup>3</sup>
    coefficient_of_thermal_expansion_1: 6.5e-06 K<sup>-1</sup>
    coefficient_of_thermal_expansion_2: 7.6e-06 K<sup>-1</sup>
    ΔP_gF: -0.0017
    acid_resistance: 51.2
    phosphate_resistance: 2.2
